1.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645 Preform Shape Optimization of Connecting Rod Using Finite Element Method and Taguchi Method Md. Israr Equbal1, Rajkumar Ohdar2, Md. Nadeem Bhat3, Suhail Ahmad lone4 1,2 Department of Forge technology, NIFFT, Ranchi 834003, India 3 Department of Foundry and Forge technology, NIFFT, Ranchi 834003, India, 4 Department of Material science and Engineering, NIFFT, Ranchi, 834003, IndiaABSTRACT : Preform design in forging processes is an important aspect for improving the forging quality and decreasingthe production cost. The objective of this paper is to obtain an optimal perform shape in the consideration of the influence ofthe metal flow deformation in closed die forging process. Finite element method based DEFORMTM 3D software inconjunction with Taguchi method has been used to simulate the closed die forging process and then performing a series ofoptimization iterations in order to obtain the optimal shape of the billet based on forging load minimization. The goal of thesimulation and optimization process is to minimize the forging load and produce defect-free forgings. The optimal shape ofthe billet that gives minimum forging load with complete die filling was obtained after several optimization iterations. Theapproach used in this study could be extended to the optimization of more complicated forging products.Keywords: Preform, Hot forging, Optimization, Finite element analysis, Taguchi method. I. INTRODUCTION In the forging process of complicated parts, the selection of appropriate preform shapes is crucial. The preformdesign in metal forging plays a key role in improving product quality, such as ensuring defect-free property and proper metalflow. In addition, it may produce more uniform strain distribution through the final forging product. Thus, the metallurgicaland mechanical properties reduce the material waste and less die wear may be achieved [1]. In designing this process,preform shape, final shape and material behaviour should be contemplated in a way to fill the die cavity completely.Furthermore, the designer should regard the process not causing any defect or undesirable properties. Main purpose of thepreform design process is achieving the following:· Assuring the metal flow without any defect and appropriately filling of the die.· Minimizing the material wastes in the flash.· Minimizing the die wear.·Obtaining the desirable grain flow and suitable mechanical properties. Traditionally, forging process design and forging process plan has employed trial & error methods which are a timeconsuming process and expensive. However, in the recent years a significant increase of computer and numerical simulationsare reported based on finite element (FE) analysis of forging process. Moreover, traditional techniques have been substitutedinto numerically based analysis. Therefore, more robust and efficient computer based approaches has been introducedrecently. As a result, a large number of investigations have been reported by different scientists in the preform design field. Zhao G. et al. [2] apply a method, which employs an alternative boundary node release criterion in the FEMsimulation of a backward deformation of forging processes. The method makes use of the shape complexity factor, whichprovides an effective measure of forging difficulty. Bramley [3] initiated a reversed method by Upper Bound ElementalTechnique (UBET) and has attained the preform shape by reversing the velocity field direction to a minimum amount forwhole of the energy distribution rate which optimized by contact conditions. Biglari et al. [4] succeed to design optimumaxisymmetric forging preforms by combining the backward tracing and fuzzy logic concepts. A new approach is introducedby Yiguo, L., et al. [5] for pre-form design called Simulation Block Technique (SBT) in which, the two half-parts of theforging die is imaginarily separated from their closed position, they move backward from each other in opposite direction ofthe forward (normal) forging process, so that the initial billet or a pre-form can be obtained, the model incorporates the useof UBET. Kang, B., S., et al. [6] presented pre-form shapes design in forging of rib-web shaped plane-strain parts weredesigned using rigid-plastic finite element method in order to obtain flash-less part. The preform was obtained by changingthe aspect ratio- the height to width ratios of the rib geometry used in the analysis. An optimization approach for the designof intermediate forging die shapes using backward deformation simulation and design optimization was developed by Han,C., S., et al. [7]. This approach could determine the pre-form die shapes from the final part shape by imposing constrains onthe plastic deformation of the material. In this paper computer simulation of the connecting rod using DEFORM (DesignEnvironment for Forming) is adopted for the purpose of optimizing the perform shape. Deform is a Finite Element Method(FEM) based process simulation system designed to analyze various forming and heat treatment processes used by metalforming and related industries. By simulating manufacturing processes on a computer, this advanced tool allows designerand engineers to Reduce the need for costly shop floor trails and redesign of tooling and process. Improve tool and die design to reduce production and material costs. Shorten lead-time in bringing a new product to market. www.ijmer.com 4532 | Page
2.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645 II. METHODOLOGY The main objective of closed die forging are complete die filling without defects viz. cracks, fold-over, wrinkleswith minimum forging load. The goal of the simulation is to find out the shape of the billet that leads to a minimum forgingload and complete die filling without any defects. Taguchi‟s experimental method is utilized to design the process parametercombinations to identify the relative influence of each parameter considered in the study. Study of the influence of designrelated variables on output performance characteristics are time consuming and costly during the real-time forging process. Whereas finite element method (FEM) based simulation software permits simulation of the system in solving linearand non-linear problems in a cost effective and timely manner. In this paper the effect of design parameters viz. flashthickness, flash width, corner radii and fillet radii on perform has been studied in order to obtain minimum forging load withcomplete die filling along with minimum material loss by using FEM based DEFORMTM 3D V6.1 to simulate and validatethe optimum result. For simulation purpose 3-D modeling software CATIA V5 is used to model part and dies. Final part andits die are as shown in Fig. 1 and Fig. 2. Dies and billets are drawn in such a manner that they are Z-axis aligned. AsDEFORMTM accepts only ‘.STL’ files, upper die, lower die and billets are saved with ‘STL’ extension. Figure 1: 3D CAD model of connecting rod Figure 2: Die of Connecting rodThe material of connecting rod is AISI 1045 alloy steel, whereas AISI-H-13 die steel is used as die material and theirproperties are given in Table I. Table I: Material Properties Property Component Die Units Density 7870 7800 Kg/m3 s Poisson‟ Ratio 0.29 0.3 --- Elastic modulus 200 210 GPa Tensile strength 585 1990 MPa Yield strength 505 1650 MPa Hardness 84 45 HRC Thermal conductivity 51.9 24.6 W/m-K III. DESIGN CONSIDERATIONS3.1 Determination of Stock SizeThe factors in estimating the stock size include the size and shape of the forging, method of heating and method of forging.The terms used in weight calculation areNet weight – it is the weight of forging as per the given dimension of the component.Net weight = volume of forging × density of materialVolume of forging = 45700 mm3 www.ijmer.com 4533 | Page
3.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645Density of material = 7.86×10-6 kg/mm3Net weight = 0.36 kgFlash loss – it is the loss of extra material comes out when the top and bottom die block has filled. It is determined by flashthickness and flash width. Flash loss = 15 to 20 % of the net weight = 0.20× 0.36 = 0.072Gross weight- the amount of material required to fabricate a forging.Gross weight = net weight +losses = 0.36+0.072kg = 0.43 kg3.2 Design of Flash The purpose of the flash is to control the metal flow within the die cavity. The flash normally cools faster than themain body of the forging and hence results resistance in metal flow outwards. The consequence of this flow restriction, metalis forced to take an alternative route, the path of least resistance, which normally results in filling dipper die cavities. Theflash thickness and width is directly related to the amount of waste material, acts as a pressure release valve for the almostincompressible work metal and restrict the outward flow of the metal so that remote corners and deeper cavities can be filledup. The finisher impression generally includes as provision for flash. The flash depression can be in either die or in both dies. Thus design of flash dimensions plays a vital role in metal filling. While designing for flash, care must be taken inselecting flash thickness, as thickness being small will necessitate greater energy or extra blows to bring forging to size, onthe other hand thickness being more may cause inadequate die filling. Thus a balanced condition is needed with just enoughvolume of metal to ensure that the flash thickness provided would force the work-metal to fill the impression properlywithout causing excess wear and pressure. Flash thickness is calculated by using the various formulas as given in Table II. Table II: Design of Flash Author Flash thickness Result Bruchanov & Rebelskii [8] 1 mm Thomas [9] 1.25mm Vieregge [10] 1.5 mm Neuberger & Mockel [11] 1.67mm Teterin & Tarnovski [12] 1.4 mmHere,A= plan projected area including flash land = 3950 mm 2D= equivalent diameter = 72 mmW= forging weight = 0.36 kg3.3 Fillet and Corner radii Fillets and corners are curved surface connecting ribs, bosses and webs, and are defined by their transverse section.A corner is a convex arc, which joins two intersecting sides at an external angle of more than 180°, whereas fillet is aconcave arc, which joins two intersecting sides at an external angle of less than 180°. Design of fillet and corner affect grainflow, forging pressure requirement, die wear, grain flow, amount of metal to be removed during machining, amount of cutgrain at junction and cost of dies and forgings. Proper selection of fillet and corner radii is vital in designing dies forforgings. Sharp corners must be avoided in forging design as they weaken both the dies and finished forgings. A sharpinternal corner or very small fillet in forging introduces a danger of cracking in heat treatments while the correspondingsharp external corner on the die prevents a satisfactory flow of metal in impression and may result in a defective forging.3.4 Press selection The main requirement selecting the press to produce a given forging is an estimate of the forging load. This willdepend on the material, forging temperature, forging complexity and flash and land dimension.For non circular forging (1) (2)Where, Dreduced = Reduced diameter of Non- Circular forging including flash land = 1.13(S1)1/2=72mmS1= Plan projected area of Non-Circular forging including flash land = 6130 mm2 www.ijmer.com 4534 | Page
4.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645σ= Tensile strength at forging temperature=6.5 kg/mm2b= Average width of forging including flash land = S1/Lmax =39.3 mmLmax = maximum length of forging at parting plane including flash land= 156mmP=8x(1-.001x72)x1.898x6130x6.5=561526 kg = 574 tonFor simulation work press capacity is taken 574 ton IV. TAGUCHI EXPERIMENTAL DESIGN Taguchi design of experiment is a powerful analysis tool for modeling and analyzing the influence of control factorson performance characteristics. The most important stage in this method lies in the selection of control factors. Anexhaustive literature review reveals that the optimized preform shape largely influenced by flash thickness (FT), flash width(FW), corner radius (RC), fillet radius (RF). These parameters each at three levels are considered for the present study. Theoperating conditions under which test are carried are shown in Table III. Table III: Factors and their levels Factors Symbol Level Unit 1 2 3 Flash thickness FT 1 1.5 2 mm Flash width FW 6 8 10 mm Corner radius RC 1.5 2 3 mm Fillet radius RF 2 3 5 mmThe total degree of freedom (DOF) for four factors each at three levels is 8. Therefore L9 orthogonal array [13] is selected forexperimental design and is shown in Table IV. Table IV: Taguchi Design for Preform (All dim. are in mm) Flash thickness Flash width Corner radii Fillet radii 1 6 1.5 2 1 8 2 3 1 10 3 5 1.5 6 2 5 1.5 8 3 2 1.5 10 1.5 3 2 6 3 3 2 8 1.5 5 2 10 2 2 V. PREFORM DESIGN Preform design is one of the most important aspects in metal forming process design. Pre-form impression allowsadequate metal distribution in the final impression. Thus, defect-free, complete die fill and small metal loses into flash can beachieved by a properly designed perform. If the component has varied cross-section as in case of spanner, connecting rod,break, pedal lever etc. it is necessary to reduce or increase cross sectional area of the bar at desired points with a view toimprove die life. This will necessitate the preforming operation before finishing. For better quality forging productions, caremust be taken that in the finishing impression to minimize deformation to achieve final shape. Traditionally, the preformdesign is based on empirical or approximate analysis, requiring time consuming and expensive trial-and–error. Hence it isnecessary to optimize the perform design in order to minimize the above drawbacks.The following procedure is used to design preform impression from forging drawing. The plan and the elevation of forging are laid out to full scale. An estimated outline of the flash of the forging preside is than laid out. The forging is then divided into various element based on geometric shape. Vertical lines are drawn through largest and smallest cross sectional area of each element found as above. The area of the above cross section is calculated and to each such area, cross sectional area of flash is added (flash width× flash thickness). From the base line of above measurement are plotted and connected with smooth line, then the cross sectional area of perform at each line is determined. The diameter “D” of the perform is evaluated at each element using the equation 3. D= (4xA/π) (1/2) (3)Where D – equivalent diameter A - Total area (flash area + job section area) Thereafter, the dimension D is symmetrically plotted about the reference line. These points are finally connectedwith a smooth curve as shown in Fig.3. A perform impression having this as an approximate contour can provide smooth www.ijmer.com 4535 | Page
5.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645flow of metal from blank into perform and finally finisher impression. For the present work 9 such performs and their dieswere designed for different values of flash thickness, flash width corner and fillet radii [14]. Front view Plan view Figure 3: Preform shape of Connecting rod VI. COMPUTER SIMULATION AND ANALYSIS OF THE FORGING PROCESS Main objective of this study is to investigate the effect of design parameters on preform shape. The computersimulation of hot forging process has been done to obtain the optimum perform shape. The DEFORM™-3D V6.1 softwarepackage was employed in the present research for the simulation and analysis of results. So far most FE based software thatsimulate billet forming processes that consider only plane-strain or axis symmetric deformations. Since many industrial partssuch as connecting rods have very complex geometries, the metal flow is three dimensional and cannot be properly modelledwith a two dimensional approximation. Therefore, a three dimensional simulation of the manufacturing process must beperformed to get adequate results. The commercial package DEFORM™-3D V6.1 offers the possibility of simulating threedimensional material flows of complex geometries. Main objective of this paper is to investigate the effect of process and design parameter to die performance andquality of the forged part. In this study, computer simulation of hot forging process has been done to obtain the optimumdesign and process parameters. The DEFORM™-3D V6.1 software package was employed in the present research for thesimulation and analysis. DEFORM essentially consists of three parts, described below.6.1 Pre-processor The pre-processor includes (i) an input module for iterative data input verification, (ii) an automatic meshgeneration program which creates a mesh by considering various process related parameters such as temperature, strain,strain-rate as well as die and work piece geometry; and (iii) an interpolation module that can interpolate various simulationresults of an old mesh onto a newly generated mesh. The combined and the automated use of the modules for automaticmesh generation and interpolation, called automatic remeshing, allow a continuous simulation of a forming process withoutany intervention by the user, even if several remeshings are required. This automatic remeshing capability drastically reducesthe total processing time of finite element analysis. All the input data generated in the pre-processor can be saved (i) in a textform which enables the user to access the input data through any text editor; and /or (ii) in a binary form which is used by thesimulation engine explained below.6.2 The simulation engine The actual FEM-based analysis is carried out in this portion of DEFORM. This simulation engine is based on arigid – plastic FE formulation and can handle a multiple number of billets (either dense material or porous material, orcombination of these materials) and dies (either rigid or linear elastic) with non-isothermal simulation capability. Thesimulation results are stored in binary form and accessed by the user through the post – processor.6.3 Post processor The post processor is used to display the results of the simulation in graphical or alphanumeric form. Thus,available graphic representations include (i) FE mesh; (ii) contour plots of distributions of strain, stress, temperature etc, (iii)velocity vectors, and (iv) load – stroke curves. Two other useful capabilities in the post –processor are (i) „ point tracking‟,which provides deformation histories of selected points in the workpiece throughout the deformation; and (ii) „flownet‟,which allows the user to observe the deformation of circles or rectangles „inscribed‟ on the undeformed workpiece for anydesired step through the simulation [15]. There are some assumed models in this paper, including that the plastic material model and the rigid die model areassumed. The velocity of the moving ram is kept constant. The strain rate at the first of deformation is equal to 2 S -1. All thesimulations started with 45000 elements. Table V shows the assumed models. www.ijmer.com 4536 | Page
6.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645 Table V: Operation parameters assigned to complete the simulation Problem Type Closed die hot forging Forging Equipment Mechanical press No. of elements 45000 Mesh type Tetrahedral Simulation mode Isothermal Primary die Top die Const. Envir. Temp. 200c Billet Temp. 10500c Die Temp. 3000c Friction Coeff. 0.3 with lubrication Die velocity 1.5 mm/s VII. RESULTS Simulations are run as per Taguchi experiment plan based on the experimental layout depicted in Table 4, andrespective value of forging load for each simulation run are converted into their respective S/N ratios as per equation 1 andare given in Table VI. Table VI: L9 orthogonal array with their response Exp. No. Parameters Response FT FW RC RF Forging load(N) (10^6) S/N Ratio Complete filling 1 1 6 1.5 2 7.86 -17.9085 No 2 1 8 2 3 7.29 -17.2546 No 3 1 10 3 5 9.73 -19.7623 No 4 1.5 6 2 5 3.82 -11.6413 Yes 5 1.5 8 3 2 7.53 -17.5359 No 6 1.5 10 1.5 3 6.25 -15.9176 Yes 7 2 6 3 3 3.17 -10.0212 Yes 8 2 8 1.5 5 3.47 -10.8066 Yes 9 2 10 2 2 4.01 -12.0629 No After conducting the experiments according to Taguchi‟s experimental design we observed that in experiment no. 1,2, 3 and 5 the problem of underfilling occurred and the forging load was also very high. This is due to small flash thicknessand improper value of corner and fillet radii. While during experiment no. 9 problem of underfilling occur because it hasbeen observed that material is going out in the form of flash without filling die cavity completely. Under filling Figure 4. Critical areas of underfilling during Simulation Figure 5. Comple die filling achieved during simulation www.ijmer.com 4537 | Page
7.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645 VIII. DISCUSSION Data analysis is made using MINITAB R14 software at 95% of confidence. Main effect plot (Fig. 6) is used todetermine the optimum factor levels for minimum forging load, which FT3, FW1, RC1 and RF2 are corresponding to thelargest values of S/N ratio for all control parameters. Relative influence of each factor is determined by analysis of variancemethod (ANOVA) presented in Table VII. Table VII: ANOVA Table for forging load Parameters Degree of freedom Sum of square Variance % Contribution F- value Flash thickness 2 81.234 40.617 77.1526 6.72 Flash width 2 11.966 5.983 11.3648 0.99 Corner radii - 6.797* - - - Fillet radii - 5.293* - - - Error 4 12.09 6.045 Total 8 105.29*pooled ANOVA depicts that the process parameter namely Flash thickness and Flash width are the most significantparameters affecting the Forging load. Fillet radius and corner radius shows the least contribution. It is necessary to mentionthat confidence level of 95% is used for analysis purpose, so p-value less than 0.05 will establish the significance of factor. Adequacy of analysis is carried out using Anderson–Darling (AD) test and results are illustrated in Fig. 7, whichshows that data follows normal distribution and develop procedure is suitable enough to explore the design space. Flash thickness Flash width -10 -12 -14 -16 Mean of SN ratios -18 1 2 3 1 2 3 Corner radius Fillet radius -10 -12 -14 -16 -18 1 2 3 1 2 3 Figure 6: S/N ratio response graph for forging load 99 Mean 5.903 StDev 2.358 95 N 9 90 AD 0.433 80 P-Value 0.233 70 Percent 60 50 40 30 20 10 5 1 -5 0 5 10 15 Re s idue Figure 7: Normal probability plot of residue at 95% of confidence IX. CONFIRMATION EXPERIMENT For confirmation purpose process is simulated at optimum factor level setting keeping all the simulation parameterfixed as given in Table 5. Fig. 8 shows the optimal forging load value of 2.13x106 N. At this load the complete die filling isachieved with maximum yield (Fig. 9). On comparing the simulation results with Taguchi predictive model which is 2.17 x10 6small error of 1.84 % indicate the Taguchi experimental plan has proceeded in a smooth manner. www.ijmer.com 4538 | Page
8.
International Journal of Modern Engineering Research (IJMER) www.ijmer.com Vol.2, Issue.6, July-Aug. 2012 pp-4532-4539 ISSN: 2249-6645 Figure 8: Load vs. stroke curve showing minimum forging load Figure 9: Complete die filling with maximum forging yield and without any defect X. CONCLUSION FEM-based computer simulation has been used to optimize the design parameters viz. flash thickness, flash width,corner radius and fillet radius on perform shape of connecting rod.Using Taguchi method, design parameters were optimizedindividually for forging load. In order to study the significance of the parameters in effecting the quality characteristics ofinterest i.e. forging load ANOVA has been performed. The conformation experiment was conducted by taking the optimizedvalue (output of Taguchi,s experiment) and was simulated once again. The results shows that at optimum factor level settingcomplete die filling is achieved with minimum forging load. It is found that optimization can be achieved quickly andefficiently through the use of simulation software. Modeling provides more information about the process i.e. loadrequirement and metal flow at different stages of the process. These techniques are also cheaper than performing tryouts withactual dies and equipments. Refrences[1] M. Sedighi, M. Hadi, and S. Kolahdouz, Optimization of Preform in Close Die Forging by Combination Of Neural Network and Genetic Algorithm, World Applied Sciences Journal, 7 (11), 2009, 1464-1473.[2] G. Zhao, E. Wright, R. V. Grandhi, Computer aided perform design in forging using the inverse die contact tracking method, International Journal of Machine Tools & Manufacturing, 36 (7), 1996, 755-769.[3] A. N. Bramley, Upper bound elemental technique (ubet) and ubet in 3d and tetrahedral upper bound analysis (teuba) fast method for forging simulation and preform design, Journal of Materials Processing Technology, 116, 2001, 80-83.[4] F. R. Biglari, N. P. O. Dowd and R. T. Fenner, Optimum design of forging dies using fuzzy logic in conjunction with the backward deformation method, Int. J. Mach. Tool Manuf. 38, 1998.[5] L. Yiguo and S. Sheng, Reverse Simulation using the Simulation Block Technique and its Application in the Precision Forging Process, Journal of Material Processing Technology, 63, 1997.[6] B. S. Kang, J. H. Lee, B. M. Kim and J. C. Choi, Process Design in Flashless Forging of Rib-Web Shaped Plane Strain Components by the Finite Element Method, Journal of Material Processing Technology, 47 1995.[7] C. S. Han, R.V. Grandhi and R. Srinivasan, Optimum Design of Forging Die Shape using Nonlinear Finite Element Analysis, AIAAJournal,31,1993.[8] A.N. Bruchanov and A.V. Rebelski, Closed die forging and warm forging (Verlag Technik 1995).[9] A. Thomas, Forging handbook, die design (Drop forging research association limited, Shefield 1981).[10] Vieregge, K., Contribution to flash design in closed die forging, doctoral dissertation, Technical university of Hanover 1969.[11] F. Neuberger and S. Pannasch, Material Consumption in Die Forging of Steel (Fertiegungstechnik und Betrieb 1962).[12] G.P. Teterin and I.J. Tarnovskij, Calculation of Plastic Dimensions in Forging Axisymmetric Parts in hammers (Kuznechno- Stampovochnoe proizvodstv 1968).[13] R.K. Roy, A primer on the taguchi method (Van Nostrand Reinhold, New York 1990).[14] G.D. Satish, N.K. Singh and R.K. Ohdar, Preform optimization of pad section of front axle beam using DEFORM, Journal of materials processing technology, 203, 2007, 102-106.[15] S.I. Oh, W.T. Wu, J.P. Tang and Vedharayagam, A Capabilities and applications of FEM code DEFORM, The Perspective of the developer, Journal of Material Processing Technology, 27, 1991, 25-42. www.ijmer.com 4539 | Page
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment